#------------------------------------------------------------------------------
#$Date: 2022-09-07 01:50:44 +0300 (Wed, 07 Sep 2022) $
#$Revision: 277696 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/71/11/7711179.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7711179
loop_
_publ_author_name
'Fraunhofer, Christina'
'Paul, Theresa'
'Oeckler, Oliver'
_publ_section_title
;
 Temperature-dependent Cu and Ag ion mobility and associated changes of
 transport properties in pavonite-type Cu1.4Ag0.4Bi5.4Se9
;
_journal_name_full               'Dalton Transactions'
_journal_paper_doi               10.1039/D2DT01651F
_journal_year                    2022
_chemical_formula_sum            'Ag0.8 Bi10.8 Cu2.8 Se18'
_chemical_formula_weight         3942.47
_space_group_crystal_system      monoclinic
_space_group_IT_number           12
_space_group_name_Hall           '-C 2y'
_space_group_name_H-M_alt        'C 1 2/m 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2017/1
_audit_update_record
;
2021-06-07 deposited with the CCDC.	2022-09-05 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 99.564(9)
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   13.7796(15)
_cell_length_b                   4.1972(5)
_cell_length_c                   15.3805(18)
_cell_measurement_reflns_used    10803
_cell_measurement_temperature    573(2)
_cell_measurement_theta_max      24.44
_cell_measurement_theta_min      2.08
_cell_volume                     877.18(18)
_computing_structure_refinement  'SHELXL-2017/1 (Sheldrick, 2017)'
_diffrn_ambient_temperature      573(2)
_diffrn_measured_fraction_theta_full 0.989
_diffrn_measured_fraction_theta_max 0.990
_diffrn_measurement_device_type  'Stoe Stadivari'
_diffrn_radiation_type           AgK\a
_diffrn_radiation_wavelength     0.56083
_diffrn_reflns_av_R_equivalents  0.0418
_diffrn_reflns_av_unetI/netI     0.0387
_diffrn_reflns_Laue_measured_fraction_full 0.989
_diffrn_reflns_Laue_measured_fraction_max 0.990
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            4831
_diffrn_reflns_point_group_measured_fraction_full 0.989
_diffrn_reflns_point_group_measured_fraction_max 0.990
_diffrn_reflns_theta_full        19.664
_diffrn_reflns_theta_max         20.506
_diffrn_reflns_theta_min         2.119
_exptl_absorpt_coefficient_mu    40.534
_exptl_absorpt_correction_T_max  0.4966
_exptl_absorpt_correction_T_min  0.1734
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(Blessing, 1995)'
_exptl_crystal_density_diffrn    7.463
_exptl_crystal_description       'irregular polyhedron'
_exptl_crystal_F_000             1627
_exptl_crystal_size_max          0.080
_exptl_crystal_size_mid          0.078
_exptl_crystal_size_min          0.042
_refine_diff_density_max         2.534
_refine_diff_density_min         -1.149
_refine_diff_density_rms         0.362
_refine_ls_extinction_coef       0.00151(16)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2017/1 (Sheldrick 2017)'
_refine_ls_goodness_of_fit_ref   1.028
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     75
_refine_ls_number_reflns         1012
_refine_ls_number_restraints     4
_refine_ls_restrained_S_all      1.026
_refine_ls_R_factor_all          0.0675
_refine_ls_R_factor_gt           0.0385
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0547P)²] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0846
_refine_ls_wR_factor_ref         0.0959
_reflns_Friedel_coverage         0.000
_reflns_number_gt                726
_reflns_number_total             1012
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d2dt01651f2.cif
_cod_data_source_block           CF215A_K3_300
_cod_original_sg_symbol_H-M      'C 2/m'
_cod_original_formula_sum        'Ag0.80 Bi10.80 Cu2.80 Se18'
_cod_database_code               7711179
_shelx_shelxl_version_number     2017/1
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Bi1 Bi 0.45133(6) 0.000000 0.18946(6) 0.0414(3) Uani 0.905(4) 2 d S T P . .
Ag1 Ag 0.45133(6) 0.000000 0.18946(6) 0.0414(3) Uani 0.062(6) 2 d S T P . .
Bi2 Bi 0.15178(7) 0.000000 0.06398(9) 0.0420(4) Uani 0.795(4) 2 d S T P . .
Ag2 Ag 0.15178(7) 0.000000 0.06398(9) 0.0420(4) Uani 0.138(6) 2 d S T P . .
Cu2 Cu 0.142(8) 0.000000 0.014(10) 0.15(5) Uiso 0.066(4) 2 d S . P . .
Bi3 Bi 0.24325(7) 0.000000 0.62219(7) 0.0568(4) Uani 1 2 d S T P . .
Se1A Se 0.4025(4) 0.000000 0.3599(6) 0.0334(16) Uani 0.90(3) 2 d S T P . .
Se1B Se 0.385(3) 0.000000 0.325(6) 0.048(10) Uiso 0.10(3) 2 d S . P . .
Se2 Se 0.79328(15) 0.000000 0.12448(17) 0.0456(6) Uani 1 2 d S T P . .
Se3 Se 0.13831(14) 0.000000 0.45567(14) 0.0339(5) Uani 1 2 d S T P . .
Se4 Se 0.09421(15) 0.000000 0.23051(15) 0.0388(5) Uani 1 2 d S T P . .
Se5 Se 0.000000 0.500000 0.000000 0.0324(6) Uani 1 4 d S T P . .
Cu3 Cu -0.023(3) 0.000000 0.438(3) 0.102(16) Uiso 0.106(7) 2 d S . P . .
Cu4 Cu 0.452(2) 0.000000 0.535(2) 0.058(9) Uiso 0.118(8) 2 d S . P . .
Cu5 Cu 0.000000 0.314(5) 0.500000 0.065(5) Uiso 0.229(8) 2 d S . P . .
Cu6 Cu 0.4908(16) 0.000000 0.5127(13) 0.036(5) Uiso 0.180(8) 2 d S . P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cu Cu 0.3240 0.8257 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Se Se 0.2367 1.4831 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ag Ag -1.6473 0.7167 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Bi Bi -1.3494 7.2566 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Se1B Bi1 Se1A 8.5(15) . . ?
Se1B Bi1 Se4 99.0(11) . 3 ?
Se1A Bi1 Se4 93.23(11) . 3 ?
Se1B Bi1 Se4 99.0(11) . 3_545 ?
Se1A Bi1 Se4 93.23(11) . 3_545 ?
Se4 Bi1 Se4 93.76(7) 3 3_545 ?
Se1B Bi1 Se2 85.9(12) . 3_445 ?
Se1A Bi1 Se2 92.11(12) . 3_445 ?
Se4 Bi1 Se2 173.43(7) 3 3_445 ?
Se4 Bi1 Se2 89.74(4) 3_545 3_445 ?
Se1B Bi1 Se2 85.9(12) . 3_455 ?
Se1A Bi1 Se2 92.11(12) . 3_455 ?
Se4 Bi1 Se2 89.74(4) 3 3_455 ?
Se4 Bi1 Se2 173.43(7) 3_545 3_455 ?
Se2 Bi1 Se2 86.26(6) 3_445 3_455 ?
Se1B Bi1 Se5 170.2(16) . 3_545 ?
Se1A Bi1 Se5 178.69(15) . 3_545 ?
Se4 Bi1 Se5 87.66(5) 3 3_545 ?
Se4 Bi1 Se5 87.66(5) 3_545 3_545 ?
Se2 Bi1 Se5 86.93(5) 3_445 3_545 ?
Se2 Bi1 Se5 86.93(5) 3_455 3_545 ?
Cu2 Bi2 Se4 153(8) . . ?
Cu2 Bi2 Se2 109(5) . 3_455 ?
Se4 Bi2 Se2 89.09(7) . 3_455 ?
Cu2 Bi2 Se2 109(5) . 3_445 ?
Se4 Bi2 Se2 89.09(7) . 3_445 ?
Se2 Bi2 Se2 92.30(7) 3_455 3_445 ?
Cu2 Bi2 Se5 71(6) . 1_545 ?
Se4 Bi2 Se5 90.69(4) . 1_545 ?
Se2 Bi2 Se5 178.03(4) 3_455 1_545 ?
Se2 Bi2 Se5 89.65(3) 3_445 1_545 ?
Cu2 Bi2 Se5 71(6) . . ?
Se4 Bi2 Se5 90.69(4) . . ?
Se2 Bi2 Se5 89.65(3) 3_455 . ?
Se2 Bi2 Se5 178.03(4) 3_445 . ?
Se5 Bi2 Se5 88.39(3) 1_545 . ?
Cu2 Bi2 Se2 24(8) . 5_655 ?
Se4 Bi2 Se2 177.67(7) . 5_655 ?
Se2 Bi2 Se2 92.52(7) 3_455 5_655 ?
Se2 Bi2 Se2 92.52(7) 3_445 5_655 ?
Se5 Bi2 Se2 87.65(4) 1_545 5_655 ?
Se5 Bi2 Se2 87.65(4) . 5_655 ?
Bi2 Cu2 Se2 148(10) . 5_655 ?
Bi2 Cu2 Se5 95(6) . 1_545 ?
Se2 Cu2 Se5 106(4) 5_655 1_545 ?
Bi2 Cu2 Se5 95(6) . . ?
Se2 Cu2 Se5 106(4) 5_655 . ?
Se5 Cu2 Se5 95(3) 1_545 . ?
Se3 Bi3 Se1B 90.7(18) . 7_546 ?
Se3 Bi3 Se1B 90.7(18) . 7_556 ?
Se1B Bi3 Se1B 91.0(11) 7_546 7_556 ?
Se3 Bi3 Se1A 79.88(19) . 7_546 ?
Se1B Bi3 Se1A 10.8(16) 7_546 7_546 ?
Se1B Bi3 Se1A 91.9(5) 7_556 7_546 ?
Se3 Bi3 Se1A 79.88(19) . 7_556 ?
Se1B Bi3 Se1A 91.9(5) 7_546 7_556 ?
Se1B Bi3 Se1A 10.8(16) 7_556 7_556 ?
Se1A Bi3 Se1A 90.73(10) 7_546 7_556 ?
Se3 Bi3 Se3 82.23(6) . 7_556 ?
Se1B Bi3 Se3 172.9(18) 7_546 7_556 ?
Se1B Bi3 Se3 90.1(7) 7_556 7_556 ?
Se1A Bi3 Se3 162.0(2) 7_546 7_556 ?
Se1A Bi3 Se3 87.93(5) 7_556 7_556 ?
Se3 Bi3 Se3 82.23(6) . 7_546 ?
Se1B Bi3 Se3 90.1(7) 7_546 7_546 ?
Se1B Bi3 Se3 172.9(18) 7_556 7_546 ?
Se1A Bi3 Se3 87.93(5) 7_546 7_546 ?
Se1A Bi3 Se3 162.0(2) 7_556 7_546 ?
Se3 Bi3 Se3 87.86(5) 7_556 7_546 ?
Se3 Bi3 Cu3 50.4(9) . 5_556 ?
Se1B Bi3 Cu3 57.8(13) 7_546 5_556 ?
Se1B Bi3 Cu3 57.8(13) 7_556 5_556 ?
Se1A Bi3 Cu3 50.5(4) 7_546 5_556 ?
Se1A Bi3 Cu3 50.5(4) 7_556 5_556 ?
Se3 Bi3 Cu3 117.3(6) 7_556 5_556 ?
Se3 Bi3 Cu3 117.3(6) 7_546 5_556 ?
Se3 Bi3 Cu4 88.9(6) . . ?
Se1B Bi3 Cu4 134.5(6) 7_546 . ?
Se1B Bi3 Cu4 134.5(6) 7_556 . ?
Se1A Bi3 Cu4 132.59(16) 7_546 . ?
Se1A Bi3 Cu4 132.59(16) 7_556 . ?
Se3 Bi3 Cu4 44.77(11) 7_556 . ?
Se3 Bi3 Cu4 44.77(10) 7_546 . ?
Cu3 Bi3 Cu4 139.3(11) 5_556 . ?
Se1B Se1A Cu6 166(4) . 5_656 ?
Se1B Se1A Cu4 149(4) . 5_656 ?
Cu6 Se1A Cu4 16.7(7) 5_656 5_656 ?
Se1B Se1A Cu6 177(4) . . ?
Cu6 Se1A Cu6 11.0(10) 5_656 . ?
Cu4 Se1A Cu6 27.7(13) 5_656 . ?
Se1B Se1A Cu5 159.7(16) . 7_556 ?
Cu6 Se1A Cu5 19.3(4) 5_656 7_556 ?
Cu4 Se1A Cu5 28.8(7) 5_656 7_556 ?
Cu6 Se1A Cu5 19.2(4) . 7_556 ?
Se1B Se1A Cu5 159.7(16) . 3_545 ?
Cu6 Se1A Cu5 19.3(4) 5_656 3_545 ?
Cu4 Se1A Cu5 28.8(7) 5_656 3_545 ?
Cu6 Se1A Cu5 19.2(4) . 3_545 ?
Cu5 Se1A Cu5 37.0(9) 7_556 3_545 ?
Se1B Se1A Cu3 122.5(13) . 3 ?
Cu6 Se1A Cu3 55.5(10) 5_656 3 ?
Cu4 Se1A Cu3 56.3(10) 5_656 3 ?
Cu6 Se1A Cu3 56.8(10) . 3 ?
Cu5 Se1A Cu3 37.7(10) 7_556 3 ?
Cu5 Se1A Cu3 74.4(11) 3_545 3 ?
Se1B Se1A Cu3 122.5(13) . 3_545 ?
Cu6 Se1A Cu3 55.5(10) 5_656 3_545 ?
Cu4 Se1A Cu3 56.3(10) 5_656 3_545 ?
Cu6 Se1A Cu3 56.8(10) . 3_545 ?
Cu5 Se1A Cu3 74.4(11) 7_556 3_545 ?
Cu5 Se1A Cu3 37.7(10) 3_545 3_545 ?
Cu3 Se1A Cu3 110.8(19) 3 3_545 ?
Se1B Se1A Cu4 169(4) . . ?
Cu6 Se1A Cu4 25.5(11) 5_656 . ?
Cu4 Se1A Cu4 42.2(16) 5_656 . ?
Cu6 Se1A Cu4 14.5(6) . . ?
Cu5 Se1A Cu4 26.8(6) 7_556 . ?
Cu5 Se1A Cu4 26.8(5) 3_545 . ?
Cu3 Se1A Cu4 60.5(10) 3 . ?
Cu3 Se1A Cu4 60.5(10) 3_545 . ?
Se1B Se1A Bi1 39(4) . . ?
Cu6 Se1A Bi1 126.1(5) 5_656 . ?
Cu4 Se1A Bi1 109.5(9) 5_656 . ?
Cu6 Se1A Bi1 137.2(5) . . ?
Cu5 Se1A Bi1 129.31(18) 7_556 . ?
Cu5 Se1A Bi1 129.31(18) 3_545 . ?
Cu3 Se1A Bi1 107.4(10) 3 . ?
Cu3 Se1A Bi1 107.4(10) 3_545 . ?
Cu4 Se1A Bi1 151.7(8) . . ?
Se1B Se1A Bi3 84(3) . 7_546 ?
Cu6 Se1A Bi3 106.0(4) 5_656 7_546 ?
Cu4 Se1A Bi3 116.7(6) 5_656 7_546 ?
Cu6 Se1A Bi3 98.5(4) . 7_546 ?
Cu5 Se1A Bi3 115.1(4) 7_556 7_546 ?
Cu5 Se1A Bi3 88.5(3) 3_545 7_546 ?
Cu3 Se1A Bi3 140.3(11) 3 7_546 ?
Cu3 Se1A Bi3 66.3(10) 3_545 7_546 ?
Cu4 Se1A Bi3 88.3(6) . 7_546 ?
Bi1 Se1A Bi3 111.0(3) . 7_546 ?
Se1A Se1B Bi1 132(4) . . ?
Se1A Se1B Cu6 12(3) . 5_656 ?
Bi1 Se1B Cu6 120.5(16) . 5_656 ?
Se1A Se1B Cu4 25(3) . 5_656 ?
Bi1 Se1B Cu4 106.8(14) . 5_656 ?
Cu6 Se1B Cu4 13.7(7) 5_656 5_656 ?
Se1A Se1B Cu3 48.1(16) . 3 ?
Bi1 Se1B Cu3 109.1(13) . 3 ?
Cu6 Se1B Cu3 46.7(15) 5_656 3 ?
Cu4 Se1B Cu3 47.8(15) 5_656 3 ?
Se1A Se1B Cu3 48.1(16) . 3_545 ?
Bi1 Se1B Cu3 109.1(13) . 3_545 ?
Cu6 Se1B Cu3 46.7(15) 5_656 3_545 ?
Cu4 Se1B Cu3 47.8(15) 5_656 3_545 ?
Cu3 Se1B Cu3 93(3) 3 3_545 ?
Se1A Se1B Bi3 85(4) . 7_546 ?
Bi1 Se1B Bi3 125(2) . 7_546 ?
Cu6 Se1B Bi3 93(2) 5_656 7_546 ?
Cu4 Se1B Bi3 103(2) 5_656 7_546 ?
Cu3 Se1B Bi3 125(3) 3 7_546 ?
Cu3 Se1B Bi3 62.5(13) 3_545 7_546 ?
Se1A Se1B Bi3 85(4) . 7_556 ?
Bi1 Se1B Bi3 125(2) . 7_556 ?
Cu6 Se1B Bi3 93(2) 5_656 7_556 ?
Cu4 Se1B Bi3 103(2) 5_656 7_556 ?
Cu3 Se1B Bi3 62.5(13) 3 7_556 ?
Cu3 Se1B Bi3 125(3) 3_545 7_556 ?
Bi3 Se1B Bi3 91.0(11) 7_546 7_556 ?
Cu2 Se2 Bi2 93(2) 5_655 3_545 ?
Cu2 Se2 Bi2 93(2) 5_655 3 ?
Bi2 Se2 Bi2 92.30(7) 3_545 3 ?
Cu2 Se2 Bi1 87(2) 5_655 3 ?
Bi2 Se2 Bi1 176.90(6) 3_545 3 ?
Bi2 Se2 Bi1 90.72(2) 3 3 ?
Cu2 Se2 Bi1 87(2) 5_655 3_545 ?
Bi2 Se2 Bi1 90.72(2) 3_545 3_545 ?
Bi2 Se2 Bi1 176.90(6) 3 3_545 ?
Bi1 Se2 Bi1 86.26(6) 3 3_545 ?
Cu2 Se2 Bi2 7(3) 5_655 5_655 ?
Bi2 Se2 Bi2 87.48(7) 3_545 5_655 ?
Bi2 Se2 Bi2 87.48(7) 3 5_655 ?
Bi1 Se2 Bi2 91.95(6) 3 5_655 ?
Bi1 Se2 Bi2 91.95(6) 3_545 5_655 ?
Cu3 Se3 Cu4 59.6(7) . 7_546 ?
Cu3 Se3 Cu4 59.6(7) . 7_556 ?
Cu4 Se3 Cu4 117.2(14) 7_546 7_556 ?
Cu3 Se3 Cu3 48(2) . 5_556 ?
Cu4 Se3 Cu3 64.5(9) 7_546 5_556 ?
Cu4 Se3 Cu3 64.5(9) 7_556 5_556 ?
Cu3 Se3 Cu5 39.8(8) . 5_556 ?
Cu4 Se3 Cu5 28.1(8) 7_546 5_556 ?
Cu4 Se3 Cu5 90.9(9) 7_556 5_556 ?
Cu3 Se3 Cu5 38.2(7) 5_556 5_556 ?
Cu3 Se3 Cu5 39.8(8) . . ?
Cu4 Se3 Cu5 90.9(9) 7_546 . ?
Cu4 Se3 Cu5 28.1(8) 7_556 . ?
Cu3 Se3 Cu5 38.2(7) 5_556 . ?
Cu5 Se3 Cu5 63.5(8) 5_556 . ?
Cu3 Se3 Bi3 119.0(13) . . ?
Cu4 Se3 Bi3 98.0(8) 7_546 . ?
Cu4 Se3 Bi3 98.0(8) 7_556 . ?
Cu3 Se3 Bi3 71.2(12) 5_556 . ?
Cu5 Se3 Bi3 93.05(6) 5_556 . ?
Cu5 Se3 Bi3 93.05(6) . . ?
Cu3 Se3 Cu6 51.1(5) . 7_546 ?
Cu4 Se3 Cu6 12.0(6) 7_546 7_546 ?
Cu4 Se3 Cu6 106.3(9) 7_556 7_546 ?
Cu3 Se3 Cu6 52.8(5) 5_556 7_546 ?
Cu5 Se3 Cu6 16.1(4) 5_556 7_546 ?
Cu5 Se3 Cu6 79.3(6) . 7_546 ?
Bi3 Se3 Cu6 95.1(4) . 7_546 ?
Cu3 Se3 Cu6 51.1(5) . 7_556 ?
Cu4 Se3 Cu6 106.3(9) 7_546 7_556 ?
Cu4 Se3 Cu6 12.0(6) 7_556 7_556 ?
Cu3 Se3 Cu6 52.8(5) 5_556 7_556 ?
Cu5 Se3 Cu6 79.3(6) 5_556 7_556 ?
Cu5 Se3 Cu6 16.1(4) . 7_556 ?
Bi3 Se3 Cu6 95.1(4) . 7_556 ?
Cu6 Se3 Cu6 95.1(6) 7_546 7_556 ?
Cu3 Se3 Bi3 123.6(7) . 7_556 ?
Cu4 Se3 Bi3 158.2(8) 7_546 7_556 ?
Cu4 Se3 Bi3 75.2(7) 7_556 7_556 ?
Cu3 Se3 Bi3 135.49(18) 5_556 7_556 ?
Cu5 Se3 Bi3 163.4(3) 5_556 7_556 ?
Cu5 Se3 Bi3 103.2(4) . 7_556 ?
Bi3 Se3 Bi3 97.77(6) . 7_556 ?
Cu6 Se3 Bi3 166.7(4) 7_546 7_556 ?
Cu6 Se3 Bi3 87.1(3) 7_556 7_556 ?
Cu3 Se3 Bi3 123.6(7) . 7_546 ?
Cu4 Se3 Bi3 75.2(7) 7_546 7_546 ?
Cu4 Se3 Bi3 158.2(8) 7_556 7_546 ?
Cu3 Se3 Bi3 135.49(18) 5_556 7_546 ?
Cu5 Se3 Bi3 103.2(4) 5_556 7_546 ?
Cu5 Se3 Bi3 163.4(3) . 7_546 ?
Bi3 Se3 Bi3 97.77(6) . 7_546 ?
Cu6 Se3 Bi3 87.1(3) 7_546 7_546 ?
Cu6 Se3 Bi3 166.7(4) 7_556 7_546 ?
Bi3 Se3 Bi3 87.86(5) 7_556 7_546 ?
Bi2 Se4 Bi1 94.97(6) . 3_445 ?
Bi2 Se4 Bi1 94.97(6) . 3_455 ?
Bi1 Se4 Bi1 93.76(7) 3_445 3_455 ?
Cu2 Se5 Cu2 180.0 5 1_565 ?
Cu2 Se5 Cu2 95(3) 5 5_565 ?
Cu2 Se5 Cu2 85(3) 1_565 5_565 ?
Cu2 Se5 Cu2 85(3) 5 . ?
Cu2 Se5 Cu2 95(3) 1_565 . ?
Cu2 Se5 Cu2 180.0 5_565 . ?
Cu2 Se5 Bi2 15(3) 5 5 ?
Cu2 Se5 Bi2 165(3) 1_565 5 ?
Cu2 Se5 Bi2 93.4(19) 5_565 5 ?
Cu2 Se5 Bi2 86.6(19) . 5 ?
Cu2 Se5 Bi2 165(3) 5 1_565 ?
Cu2 Se5 Bi2 15(3) 1_565 1_565 ?
Cu2 Se5 Bi2 86.6(19) 5_565 1_565 ?
Cu2 Se5 Bi2 93.4(19) . 1_565 ?
Bi2 Se5 Bi2 180.00(5) 5 1_565 ?
Cu2 Se5 Bi2 93.4(19) 5 5_565 ?
Cu2 Se5 Bi2 86.6(19) 1_565 5_565 ?
Cu2 Se5 Bi2 15(3) 5_565 5_565 ?
Cu2 Se5 Bi2 165(3) . 5_565 ?
Bi2 Se5 Bi2 88.39(3) 5 5_565 ?
Bi2 Se5 Bi2 91.61(3) 1_565 5_565 ?
Cu2 Se5 Bi2 86.6(19) 5 . ?
Cu2 Se5 Bi2 93.4(19) 1_565 . ?
Cu2 Se5 Bi2 165(3) 5_565 . ?
Cu2 Se5 Bi2 15(3) . . ?
Bi2 Se5 Bi2 91.61(3) 5 . ?
Bi2 Se5 Bi2 88.39(3) 1_565 . ?
Bi2 Se5 Bi2 180.0 5_565 . ?
Cu2 Se5 Bi1 80(3) 5 3_455 ?
Cu2 Se5 Bi1 100(3) 1_565 3_455 ?
Cu2 Se5 Bi1 80(3) 5_565 3_455 ?
Cu2 Se5 Bi1 100(3) . 3_455 ?
Bi2 Se5 Bi1 93.46(3) 5 3_455 ?
Bi2 Se5 Bi1 86.54(3) 1_565 3_455 ?
Bi2 Se5 Bi1 93.46(3) 5_565 3_455 ?
Bi2 Se5 Bi1 86.54(3) . 3_455 ?
Cu2 Se5 Bi1 100(3) 5 7 ?
Cu2 Se5 Bi1 80(3) 1_565 7 ?
Cu2 Se5 Bi1 100(3) 5_565 7 ?
Cu2 Se5 Bi1 80(3) . 7 ?
Bi2 Se5 Bi1 86.54(3) 5 7 ?
Bi2 Se5 Bi1 93.46(3) 1_565 7 ?
Bi2 Se5 Bi1 86.54(3) 5_565 7 ?
Bi2 Se5 Bi1 93.46(3) . 7 ?
Bi1 Se5 Bi1 180.0 3_455 7 ?
Cu5 Cu3 Cu5 108(3) 5_556 . ?
Cu5 Cu3 Cu3 54.1(15) 5_556 5_556 ?
Cu5 Cu3 Cu3 54.1(15) . 5_556 ?
Cu5 Cu3 Se3 80.5(18) 5_556 . ?
Cu5 Cu3 Se3 80.5(18) . . ?
Cu3 Cu3 Se3 74(3) 5_556 . ?
Cu5 Cu3 Cu6 123(3) 5_556 7_556 ?
Cu5 Cu3 Cu6 16.0(6) . 7_556 ?
Cu3 Cu3 Cu6 69.5(13) 5_556 7_556 ?
Se3 Cu3 Cu6 79.7(13) . 7_556 ?
Cu5 Cu3 Cu6 16.0(6) 5_556 7_546 ?
Cu5 Cu3 Cu6 123(3) . 7_546 ?
Cu3 Cu3 Cu6 69.5(13) 5_556 7_546 ?
Se3 Cu3 Cu6 79.7(13) . 7_546 ?
Cu6 Cu3 Cu6 138(3) 7_556 7_546 ?
Cu5 Cu3 Cu4 126(3) 5_556 7_556 ?
Cu5 Cu3 Cu4 29.3(10) . 7_556 ?
Cu3 Cu3 Cu4 76.2(18) 5_556 7_556 ?
Se3 Cu3 Cu4 66.0(13) . 7_556 ?
Cu6 Cu3 Cu4 16.9(7) 7_556 7_556 ?
Cu6 Cu3 Cu4 137(2) 7_546 7_556 ?
Cu5 Cu3 Cu4 29.3(10) 5_556 7_546 ?
Cu5 Cu3 Cu4 126(3) . 7_546 ?
Cu3 Cu3 Cu4 76.2(18) 5_556 7_546 ?
Se3 Cu3 Cu4 66.0(13) . 7_546 ?
Cu6 Cu3 Cu4 137(2) 7_556 7_546 ?
Cu6 Cu3 Cu4 16.9(7) 7_546 7_546 ?
Cu4 Cu3 Cu4 129(3) 7_556 7_546 ?
Cu5 Cu3 Cu6 116(3) 5_556 3_455 ?
Cu5 Cu3 Cu6 9.1(7) . 3_455 ?
Cu3 Cu3 Cu6 62.1(12) 5_556 3_455 ?
Se3 Cu3 Cu6 86.8(14) . 3_455 ?
Cu6 Cu3 Cu6 12.0(9) 7_556 3_455 ?
Cu6 Cu3 Cu6 132(2) 7_546 3_455 ?
Cu4 Cu3 Cu6 28.5(13) 7_556 3_455 ?
Cu4 Cu3 Cu6 135(3) 7_546 3_455 ?
Cu5 Cu3 Cu6 9.1(7) 5_556 3_445 ?
Cu5 Cu3 Cu6 116(3) . 3_445 ?
Cu3 Cu3 Cu6 62.1(12) 5_556 3_445 ?
Se3 Cu3 Cu6 86.8(14) . 3_445 ?
Cu6 Cu3 Cu6 132(2) 7_556 3_445 ?
Cu6 Cu3 Cu6 12.0(9) 7_546 3_445 ?
Cu4 Cu3 Cu6 135(3) 7_556 3_445 ?
Cu4 Cu3 Cu6 28.5(13) 7_546 3_445 ?
Cu6 Cu3 Cu6 123(2) 3_455 3_445 ?
Cu5 Cu3 Se3 72.2(16) 5_556 5_556 ?
Cu5 Cu3 Se3 72.2(16) . 5_556 ?
Cu3 Cu3 Se3 59(2) 5_556 5_556 ?
Se3 Cu3 Se3 132(2) . 5_556 ?
Cu6 Cu3 Se3 83.6(14) 7_556 5_556 ?
Cu6 Cu3 Se3 83.6(14) 7_546 5_556 ?
Cu4 Cu3 Se3 100.3(16) 7_556 5_556 ?
Cu4 Cu3 Se3 100.3(16) 7_546 5_556 ?
Cu6 Cu3 Se3 71.8(12) 3_455 5_556 ?
Cu6 Cu3 Se3 71.8(12) 3_445 5_556 ?
Cu5 Cu3 Se1A 68.5(7) 5_556 3_445 ?
Cu5 Cu3 Se1A 165(3) . 3_445 ?
Cu3 Cu3 Se1A 120.8(13) 5_556 3_445 ?
Se3 Cu3 Se1A 112.3(12) . 3_445 ?
Cu6 Cu3 Se1A 165(2) 7_556 3_445 ?
Cu6 Cu3 Se1A 55.4(6) 7_546 3_445 ?
Cu4 Cu3 Se1A 162(2) 7_556 3_445 ?
Cu4 Cu3 Se1A 57.6(8) 7_546 3_445 ?
Cu6 Cu3 Se1A 161(2) 3_455 3_445 ?
Cu6 Cu3 Se1A 59.7(6) 3_445 3_445 ?
Se3 Cu3 Se1A 93.3(12) 5_556 3_445 ?
Cu6 Cu4 Cu6 9(4) . 5_656 ?
Cu6 Cu4 Cu5 40.9(15) . 7_556 ?
Cu6 Cu4 Cu5 40.7(15) 5_656 7_556 ?
Cu6 Cu4 Cu5 40.9(15) . 3_545 ?
Cu6 Cu4 Cu5 40.7(15) 5_656 3_545 ?
Cu5 Cu4 Cu5 81(3) 7_556 3_545 ?
Cu6 Cu4 Cu4 6(2) . 5_656 ?
Cu6 Cu4 Cu4 3.3(13) 5_656 5_656 ?
Cu5 Cu4 Cu4 40.6(14) 7_556 5_656 ?
Cu5 Cu4 Cu4 40.6(15) 3_545 5_656 ?
Cu6 Cu4 Cu3 75.5(19) . 7_556 ?
Cu6 Cu4 Cu3 78.8(16) 5_656 7_556 ?
Cu5 Cu4 Cu3 41.3(14) 7_556 7_556 ?
Cu5 Cu4 Cu3 115(3) 3_545 7_556 ?
Cu4 Cu4 Cu3 77.6(16) 5_656 7_556 ?
Cu6 Cu4 Cu3 75.5(19) . 7_546 ?
Cu6 Cu4 Cu3 78.8(16) 5_656 7_546 ?
Cu5 Cu4 Cu3 115(3) 7_556 7_546 ?
Cu5 Cu4 Cu3 41.3(14) 3_545 7_546 ?
Cu4 Cu4 Cu3 77.6(16) 5_656 7_546 ?
Cu3 Cu4 Cu3 129(3) 7_556 7_546 ?
Cu6 Cu4 Se1A 72(4) . 5_656 ?
Cu6 Cu4 Se1A 81.2(19) 5_656 5_656 ?
Cu5 Cu4 Se1A 80.9(16) 7_556 5_656 ?
Cu5 Cu4 Se1A 80.9(16) 3_545 5_656 ?
Cu4 Cu4 Se1A 78(2) 5_656 5_656 ?
Cu3 Cu4 Se1A 66.1(14) 7_556 5_656 ?
Cu3 Cu4 Se1A 66.1(14) 7_546 5_656 ?
Cu6 Cu4 Se3 118.6(13) . 7_546 ?
Cu6 Cu4 Se3 116.2(9) 5_656 7_546 ?
Cu5 Cu4 Se3 154(2) 7_556 7_546 ?
Cu5 Cu4 Se3 78.0(9) 3_545 7_546 ?
Cu4 Cu4 Se3 117.2(11) 5_656 7_546 ?
Cu3 Cu4 Se3 164(2) 7_556 7_546 ?
Cu3 Cu4 Se3 54.5(11) 7_546 7_546 ?
Se1A Cu4 Se3 109.9(9) 5_656 7_546 ?
Cu6 Cu4 Se3 118.6(13) . 7_556 ?
Cu6 Cu4 Se3 116.2(9) 5_656 7_556 ?
Cu5 Cu4 Se3 78.0(9) 7_556 7_556 ?
Cu5 Cu4 Se3 154(2) 3_545 7_556 ?
Cu4 Cu4 Se3 117.2(11) 5_656 7_556 ?
Cu3 Cu4 Se3 54.5(11) 7_556 7_556 ?
Cu3 Cu4 Se3 164(2) 7_546 7_556 ?
Se1A Cu4 Se3 109.9(9) 5_656 7_556 ?
Se3 Cu4 Se3 117.2(14) 7_546 7_556 ?
Cu6 Cu4 Cu3 62(2) . 3_545 ?
Cu6 Cu4 Cu3 58.4(11) 5_656 3_545 ?
Cu5 Cu4 Cu3 98(2) 7_556 3_545 ?
Cu5 Cu4 Cu3 25.4(14) 3_545 3_545 ?
Cu4 Cu4 Cu3 59.6(13) 5_656 3_545 ?
Cu3 Cu4 Cu3 137.2(16) 7_556 3_545 ?
Cu3 Cu4 Cu3 45(2) 7_546 3_545 ?
Se1A Cu4 Cu3 102.3(14) 5_656 3_545 ?
Se3 Cu4 Cu3 57.8(9) 7_546 3_545 ?
Se3 Cu4 Cu3 146.2(18) 7_556 3_545 ?
Cu6 Cu4 Cu3 62(2) . 3 ?
Cu6 Cu4 Cu3 58.4(11) 5_656 3 ?
Cu5 Cu4 Cu3 25.4(14) 7_556 3 ?
Cu5 Cu4 Cu3 98(2) 3_545 3 ?
Cu4 Cu4 Cu3 59.6(13) 5_656 3 ?
Cu3 Cu4 Cu3 45(2) 7_556 3 ?
Cu3 Cu4 Cu3 137.2(16) 7_546 3 ?
Se1A Cu4 Cu3 102.3(14) 5_656 3 ?
Se3 Cu4 Cu3 146.2(18) 7_546 3 ?
Se3 Cu4 Cu3 57.8(9) 7_556 3 ?
Cu3 Cu4 Cu3 106(2) 3_545 3 ?
Cu6 Cu5 Cu6 35(3) 3_455 7_556 ?
Cu6 Cu5 Cu4 67(3) 3_455 7_556 ?
Cu6 Cu5 Cu4 32.6(10) 7_556 7_556 ?
Cu6 Cu5 Cu4 32.6(10) 3_455 3_455 ?
Cu6 Cu5 Cu4 67(3) 7_556 3_455 ?
Cu4 Cu5 Cu4 99(3) 7_556 3_455 ?
Cu6 Cu5 Cu5 17.7(15) 3_455 5_566 ?
Cu6 Cu5 Cu5 17.7(15) 7_556 5_566 ?
Cu4 Cu5 Cu5 49.4(14) 7_556 5_566 ?
Cu4 Cu5 Cu5 49.4(15) 3_455 5_566 ?
Cu6 Cu5 Cu3 153(2) 3_455 . ?
Cu6 Cu5 Cu3 131(2) 7_556 . ?
Cu4 Cu5 Cu3 109(2) 7_556 . ?
Cu4 Cu5 Cu3 136(2) 3_455 . ?
Cu5 Cu5 Cu3 144.1(15) 5_566 . ?
Cu6 Cu5 Cu3 131(2) 3_455 5_556 ?
Cu6 Cu5 Cu3 153(2) 7_556 5_556 ?
Cu4 Cu5 Cu3 136(2) 7_556 5_556 ?
Cu4 Cu5 Cu3 109(2) 3_455 5_556 ?
Cu5 Cu5 Cu3 144.1(16) 5_566 5_556 ?
Cu3 Cu5 Cu3 72(3) . 5_556 ?
Cu6 Cu5 Se1A 64.7(15) 3_455 7_556 ?
Cu6 Cu5 Se1A 79.8(16) 7_556 7_556 ?
Cu4 Cu5 Se1A 85.6(16) 7_556 7_556 ?
Cu4 Cu5 Se1A 70.4(16) 3_455 7_556 ?
Cu5 Cu5 Se1A 71.5(4) 5_566 7_556 ?
Cu3 Cu5 Se1A 142.4(18) . 7_556 ?
Cu3 Cu5 Se1A 73.8(15) 5_556 7_556 ?
Cu6 Cu5 Se1A 79.8(16) 3_455 3_455 ?
Cu6 Cu5 Se1A 64.7(15) 7_556 3_455 ?
Cu4 Cu5 Se1A 70.4(16) 7_556 3_455 ?
Cu4 Cu5 Se1A 85.6(16) 3_455 3_455 ?
Cu5 Cu5 Se1A 71.5(4) 5_566 3_455 ?
Cu3 Cu5 Se1A 73.8(15) . 3_455 ?
Cu3 Cu5 Se1A 142.4(18) 5_556 3_455 ?
Se1A Cu5 Se1A 143.0(9) 7_556 3_455 ?
Cu6 Cu5 Se3 136.1(17) 3_455 . ?
Cu6 Cu5 Se3 106.3(14) 7_556 . ?
Cu4 Cu5 Se3 74.0(12) 7_556 . ?
Cu4 Cu5 Se3 163.8(17) 3_455 . ?
Cu5 Cu5 Se3 121.7(4) 5_566 . ?
Cu3 Cu5 Se3 59.7(17) . . ?
Cu3 Cu5 Se3 69.6(16) 5_556 . ?
Se1A Cu5 Se3 94.35(13) 7_556 . ?
Se1A Cu5 Se3 104.93(15) 3_455 . ?
Cu6 Cu5 Se3 106.3(14) 3_455 5_556 ?
Cu6 Cu5 Se3 136.1(17) 7_556 5_556 ?
Cu4 Cu5 Se3 163.8(16) 7_556 5_556 ?
Cu4 Cu5 Se3 74.0(13) 3_455 5_556 ?
Cu5 Cu5 Se3 121.7(4) 5_566 5_556 ?
Cu3 Cu5 Se3 69.6(16) . 5_556 ?
Cu3 Cu5 Se3 59.7(17) 5_556 5_556 ?
Se1A Cu5 Se3 104.93(15) 7_556 5_556 ?
Se1A Cu5 Se3 94.35(13) 3_455 5_556 ?
Se3 Cu5 Se3 116.5(8) . 5_556 ?
Cu6 Cu5 Cu5 162.3(15) 3_455 5_556 ?
Cu6 Cu5 Cu5 162.3(15) 7_556 5_556 ?
Cu4 Cu5 Cu5 130.6(14) 7_556 5_556 ?
Cu4 Cu5 Cu5 130.6(15) 3_455 5_556 ?
Cu5 Cu5 Cu5 180.000(16) 5_566 5_556 ?
Cu3 Cu5 Cu5 35.9(15) . 5_556 ?
Cu3 Cu5 Cu5 35.9(15) 5_556 5_556 ?
Se1A Cu5 Cu5 108.5(4) 7_556 5_556 ?
Se1A Cu5 Cu5 108.5(4) 3_455 5_556 ?
Se3 Cu5 Cu5 58.3(4) . 5_556 ?
Se3 Cu5 Cu5 58.3(4) 5_556 5_556 ?
Cu6 Cu6 Cu4 159(8) 5_656 . ?
Cu6 Cu6 Cu5 72.3(15) 5_656 3_545 ?
Cu4 Cu6 Cu5 106.6(16) . 3_545 ?
Cu6 Cu6 Cu5 72.3(15) 5_656 7_556 ?
Cu4 Cu6 Cu5 106.6(16) . 7_556 ?
Cu5 Cu6 Cu5 145(3) 3_545 7_556 ?
Cu6 Cu6 Cu4 12(5) 5_656 5_656 ?
Cu4 Cu6 Cu4 171(4) . 5_656 ?
Cu5 Cu6 Cu4 72.7(15) 3_545 5_656 ?
Cu5 Cu6 Cu4 72.7(15) 7_556 5_656 ?
Cu6 Cu6 Se1A 110(5) 5_656 5_656 ?
Cu4 Cu6 Se1A 91(4) . 5_656 ?
Cu5 Cu6 Se1A 95.9(16) 3_545 5_656 ?
Cu5 Cu6 Se1A 95.9(15) 7_556 5_656 ?
Cu4 Cu6 Se1A 97.9(18) 5_656 5_656 ?
Cu6 Cu6 Cu3 100(2) 5_656 7_556 ?
Cu4 Cu6 Cu3 87.6(19) . 7_556 ?
Cu5 Cu6 Cu3 160(2) 3_545 7_556 ?
Cu5 Cu6 Cu3 33.1(15) 7_556 7_556 ?
Cu4 Cu6 Cu3 95.6(15) 5_656 7_556 ?
Se1A Cu6 Cu3 69.1(13) 5_656 7_556 ?
Cu6 Cu6 Cu3 100(2) 5_656 7_546 ?
Cu4 Cu6 Cu3 87.6(19) . 7_546 ?
Cu5 Cu6 Cu3 33.1(15) 3_545 7_546 ?
Cu5 Cu6 Cu3 160(2) 7_556 7_546 ?
Cu4 Cu6 Cu3 95.6(15) 5_656 7_546 ?
Se1A Cu6 Cu3 69.1(13) 5_656 7_546 ?
Cu3 Cu6 Cu3 138(3) 7_556 7_546 ?
Cu6 Cu6 Cu3 68(2) 5_656 3_545 ?
Cu4 Cu6 Cu3 104(2) . 3_545 ?
Cu5 Cu6 Cu3 18.2(15) 3_545 3_545 ?
Cu5 Cu6 Cu3 137(2) 7_556 3_545 ?
Cu4 Cu6 Cu3 72.7(13) 5_656 3_545 ?
Se1A Cu6 Cu3 114.1(13) 5_656 3_545 ?
Cu3 Cu6 Cu3 168.0(9) 7_556 3_545 ?
Cu3 Cu6 Cu3 48(2) 7_546 3_545 ?
Cu6 Cu6 Cu3 68(2) 5_656 3 ?
Cu4 Cu6 Cu3 104(2) . 3 ?
Cu5 Cu6 Cu3 137(2) 3_545 3 ?
Cu5 Cu6 Cu3 18.2(15) 7_556 3 ?
Cu4 Cu6 Cu3 72.7(12) 5_656 3 ?
Se1A Cu6 Cu3 114.1(13) 5_656 3 ?
Cu3 Cu6 Cu3 48(2) 7_556 3 ?
Cu3 Cu6 Cu3 168.0(9) 7_546 3 ?
Cu3 Cu6 Cu3 123(2) 3_545 3 ?
Cu6 Cu6 Se1A 59(5) 5_656 . ?
Cu4 Cu6 Se1A 100(4) . . ?
Cu5 Cu6 Se1A 81.0(15) 3_545 . ?
Cu5 Cu6 Se1A 81.0(15) 7_556 . ?
Cu4 Cu6 Se1A 71.1(16) 5_656 . ?
Se1A Cu6 Se1A 169.0(10) 5_656 . ?
Cu3 Cu6 Se1A 111.1(13) 7_556 . ?
Cu3 Cu6 Se1A 111.1(13) 7_546 . ?
Cu3 Cu6 Se1A 63.5(12) 3_545 . ?
Cu3 Cu6 Se1A 63.5(12) 3 . ?
Cu6 Cu6 Se1B 113(5) 5_656 5_656 ?
Cu4 Cu6 Se1B 88(4) . 5_656 ?
Cu5 Cu6 Se1B 96.7(16) 3_545 5_656 ?
Cu5 Cu6 Se1B 96.7(16) 7_556 5_656 ?
Cu4 Cu6 Se1B 101(2) 5_656 5_656 ?
Se1A Cu6 Se1B 2.8(9) 5_656 5_656 ?
Cu3 Cu6 Se1B 69.0(13) 7_556 5_656 ?
Cu3 Cu6 Se1B 69.0(13) 7_546 5_656 ?
Cu3 Cu6 Se1B 114.8(13) 3_545 5_656 ?
Cu3 Cu6 Se1B 114.8(13) 3 5_656 ?
Se1A Cu6 Se1B 171.8(13) . 5_656 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Bi1 Se1B 2.41(8) . ?
Bi1 Se1A 2.813(7) . ?
Bi1 Se4 2.8750(16) 3 ?
Bi1 Se4 2.8750(16) 3_545 ?
Bi1 Se2 3.0698(17) 3_445 ?
Bi1 Se2 3.0698(17) 3_455 ?
Bi1 Se5 3.0969(10) 3_545 ?
Bi2 Cu2 0.76(15) . ?
Bi2 Se4 2.804(3) . ?
Bi2 Se2 2.9101(18) 3_455 ?
Bi2 Se2 2.9101(18) 3_445 ?
Bi2 Se5 3.0104(8) 1_545 ?
Bi2 Se5 3.0104(8) . ?
Bi2 Se2 3.115(3) 5_655 ?
Cu2 Se2 2.44(14) 5_655 ?
Cu2 Se5 2.85(8) 1_545 ?
Cu2 Se5 2.85(8) . ?
Bi3 Se3 2.724(2) . ?
Bi3 Se1B 2.94(3) 7_546 ?
Bi3 Se1B 2.94(3) 7_556 ?
Bi3 Se1A 2.949(3) 7_546 ?
Bi3 Se1A 2.949(3) 7_556 ?
Bi3 Se3 3.0250(15) 7_556 ?
Bi3 Se3 3.0250(15) 7_546 ?
Bi3 Cu3 3.03(5) 5_556 ?
Bi3 Cu4 3.37(4) . ?
Se1A Se1B 0.56(8) . ?
Se1A Cu6 2.24(2) 5_656 ?
Se1A Cu4 2.36(3) 5_656 ?
Se1A Cu6 2.46(2) . ?
Se1A Cu5 2.469(11) 7_556 ?
Se1A Cu5 2.469(11) 3_545 ?
Se1A Cu3 2.55(3) 3 ?
Se1A Cu3 2.55(3) 3_545 ?
Se1A Cu4 2.66(4) . ?
Se1B Cu6 2.79(9) 5_656 ?
Se1B Cu4 2.85(9) 5_656 ?
Se1B Cu3 2.89(7) 3 ?
Se1B Cu3 2.89(7) 3_545 ?
Se3 Cu3 2.19(5) . ?
Se3 Cu4 2.459(18) 7_546 ?
Se3 Cu4 2.459(18) 7_556 ?
Se3 Cu3 2.46(5) 5_556 ?
Se3 Cu5 2.502(10) 5_556 ?
Se3 Cu5 2.502(10) . ?
Se3 Cu6 2.845(14) 7_546 ?
Se3 Cu6 2.845(14) 7_556 ?
Cu3 Cu5 1.62(3) 5_556 ?
Cu3 Cu5 1.62(3) . ?
Cu3 Cu3 1.90(10) 5_556 ?
Cu3 Cu6 2.25(2) 7_556 ?
Cu3 Cu6 2.25(2) 7_546 ?
Cu3 Cu4 2.32(3) 7_556 ?
Cu3 Cu4 2.32(3) 7_546 ?
Cu3 Cu6 2.38(3) 3_455 ?
Cu3 Cu6 2.38(3) 3_445 ?
Cu4 Cu6 0.68(3) . ?
Cu4 Cu6 1.16(5) 5_656 ?
Cu4 Cu5 1.20(3) 7_556 ?
Cu4 Cu5 1.20(3) 3_545 ?
Cu4 Cu4 1.83(7) 5_656 ?
Cu5 Cu6 0.822(17) 3_455 ?
Cu5 Cu6 0.822(17) 7_556 ?
Cu5 Cu5 1.57(4) 5_566 ?
Cu5 Cu5 2.63(4) 5_556 ?
Cu6 Cu6 0.50(4) 5_656 ?
